TB-0703 — Recommended Procedures for Batching and Mixing FORCE 10,000D® Concrete Technical Bulletin
The key to producing high quality, high performance concrete with FORCE 10,000D® is thorough mixing. It is essential that FORCE 10,000D® is uniformly distributed throughout the concrete mixture and the densified silica fume broken up. This technical bulletin offers recommendations for batching and mixing FORCE 10,000D® concrete. The basic recommendations provided by ACI 304, “Guide for Measuring, Mixing, Transporting and Placing Concrete” should be followed for producing concrete; however, FORCE 10,000D® requires further batching and mixing details that will be discussed in this technical bulletin. The “Silica Fume User’s Manual” by the Silica Fume Association and printed by the Federal Highway Administration, FHWA-IF-05-016, contains good information for batching and mixing silica fume concrete.
FORCE 10,000D® is available as a dry-densified powder, both in bulk and bagged. The bulk material is delivered into a silo at the concrete producer and added to the mix similar to cement. The bagged material is added, by hand, unopened t o the mixer since the bags are designed to disintegrate during mixing, or opened and then poured into the mixer.
Batching and Mixing
FORCE 10,000D® as bulk silica fume should be weighed just like cement. However, care should be taken to avoid weighing errors due to the smaller amount of Force 10,000 as compared to the larger quantities of other mix ingredients. Add the FORCE 10,000D® with the other cementitious material and other concrete ingredients. Never add the FORCE 10,000D® first into an empty drum or mixer with only water in the drum. Do not yet add the superplasticizer. Turn the mixer for 100 revolutions at mixing (charging) speed at a concrete slump of 50 to 100 mm (2 in. to 4 in.). This lower slump will eliminate the potential for silica fume or cement balls from forming and allow for uniform dispersion. After this mixing has taken place, add the superplasticizer to bring the mix up to the desired slump by mixing an additional 70 revolutions at mixing speed.
FORCE 10,000D® is also sold in 11.3 kg (25 lbs) repulpable bags. These bags are designed to disintegrate in a mixer due to grinding and wetting of the paper during the mixing process. Note the condition of the bags before using. If the bags are wet, do not use them. Wet silica fume will not disperse correctly. Start by counting and setting aside the number of bags necessary for each truck. As an example, if the specification calls for a 5% replacement on a 385 kg/m3 (650 lbs/yd3) mix, then 13 bags of FORCE 10,000D® will be required for a 8 m3 (10 yd3) truck.
650 lbs/yd3 X 0.05 = 32.5 lbs/yd3 X 10 yd3 per truck = 325 lbs of FORCE 10,000D®. 325 lbs / 25 lbs/bag of FORCE 10,000D® = 13 bags.
385 kg/m3 X 0.05 = 19.3 kg/m3 X 8 m3 per truck = 154 kg of FORCE 10,000D®. 154 kg / 11.3 kg/bag of FORCE 10,000D® = 13.6 bags. Use 14 bags.
Add the cement, aggregates and water to the mixer, but not the superplasticizer. Add the bagged FORCE 10,000D® to the drum. Never add the FORCE 10,000D® first into an empty drum or mixer with only water in the drum. Mix for 100 revolutions at mixing speed. Add the superplasticizer to bring the concrete up to the required slump and mix for another 70 revolutions.
There are instances when the bags may not completely disintegrate. This can occur in low water/cementitious mixes, mixes with coarse aggregate of 13 mm (½ in.) or less, rounded aggregate, or in pan mixers. If the concrete producer is concerned that this may occur, run a test with the proposed mix and view the results. If the bags do not disintegrate, then during concrete production open the bags and empty them into the mixer when the drum is not moving. Discard the bags.
gcpat.com | North America Customer Service: 1 877-4AD-MIX1 (1 877-423-6491)
We hope the information here will be helpful. It is based on data and knowledge considered to be true and accurate and is offered for consideration, investigation and verification by the user, but we do not warrant the results to be obtained. Please read all statements, recommendations and suggestions in conjunction with our conditions of sale, which apply to all goods supplied by us. No statement, recommendation, or suggestion is intended for any use that would infringe any patent, copyright, or other third party right.
FORCE 10000D is a trademark, which may be registered in the United States and/or other countries, of GCP Applied Technologies Inc. This trademark list has been compiled using available published information as of the publication date and may not accurately reflect current trademark ownership or status.
© Copyright 2018 GCP Applied Technologies Inc. All rights reserved.
GCP Applied Technologies Inc., 62 Whittemore Avenue, Cambridge, MA 02140 USA.
In Canada, 294 Clements Road, West, Ajax, Ontario, Canada L1S 3C6.
This document is only current as of the last updated date stated below and is valid only for use in the United States. It is important that you always refer to the currently available information at the URL below to provide the most current product information at the time of use. Additional literature such as Contractor Manuals, Technical Bulletins, Detail Drawings and detailing recommendations and other relevant documents are also available on www.gcpat.com. Information found on other websites must not be relied upon, as they may not be up-to-date or applicable to the conditions in your location and we do not accept any responsibility for their content. If there are any conflicts or if you need more information, please contact GCP Customer Service.
Last Updated: 2018-11-29